General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.47 - 7.7 g/cm³ Show Material materials with Density of 7.47 - 7.7 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | 20.0 °C | 218 GPa Show Material materials with Elastic modulus of 218 GPa | |

100.0 °C | 213 GPa Show Material materials with Elastic modulus of 213 GPa | ||

200.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa | ||

300.0 °C | 198 GPa Show Material materials with Elastic modulus of 198 GPa | ||

400.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | ||

500.0 °C | 180 GPa Show Material materials with Elastic modulus of 180 GPa | ||

600.0 °C | 167 GPa Show Material materials with Elastic modulus of 167 GPa | ||

700.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | ||

Elongation | 20.0 °C | 10 - 15 % Show Material materials with Elongation of 10 - 15 % | |

Elongation A80 | 20.0 °C | 13 % Show Material materials with Elongation A80 of 13 % | |

Hardness, Brinell | 20.0 °C | 223 [-] Show Material materials with Hardness, Brinell of 223 [-] | |

Poisson's ratio | 23.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | Typical for Ferritic Stainless Steel |

Shear modulus | 23.0 °C | 77 GPa Show Material materials with Shear modulus of 77 GPa | Typical for Ferritic Stainless Steel |

Tensile strength | 20.0 °C | 520 - 720 MPa Show Material materials with Tensile strength of 520 - 720 MPa | |

Yield strength Rp0.2 | 20.0 °C | 280 MPa Show Material materials with Yield strength Rp0.2 of 280 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 20.0 °C | 9.9E-6 1/K Show Material materials with Coefficient of thermal expansion of 9.9E-6 1/K | |

100.0 °C | 1.03E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.03E-5 1/K | ||

200.0 °C | 1.05E-5 - 1.07E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 - 1.07E-5 1/K | ||

300.0 °C | 1.11E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.11E-5 1/K | ||

400.0 °C | 1.15E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.15E-5 1/K | ||

500.0 °C | 1.18E-5 - 1.2E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.18E-5 - 1.2E-5 1/K | ||

600.0 °C | 1.2E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.2E-5 1/K | ||

700.0 °C | 1.24E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.24E-5 1/K | ||

800.0 °C | 1.2E-5 - 1.29E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.2E-5 - 1.29E-5 1/K | ||

900.0 °C | 1.34E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.34E-5 1/K | ||

1000.0 °C | 1.35E-5 - 1.4E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.35E-5 - 1.4E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 1000 °C Show Material materials with Max service temperature, long of 0 - 1000 °C | ||

Melting point | 1425 - 1530 °C Show Material materials with Melting point of 1425 - 1530 °C | Typical for Ferritic Stainless Steel | |

Specific heat capacity | 20.0 °C | 457 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 457 - 500 J/(kg·K) | |

100.0 °C | 498 J/(kg·K) Show Material materials with Specific heat capacity of 498 J/(kg·K) | ||

200.0 °C | 534 J/(kg·K) Show Material materials with Specific heat capacity of 534 J/(kg·K) | ||

300.0 °C | 555 J/(kg·K) Show Material materials with Specific heat capacity of 555 J/(kg·K) | ||

400.0 °C | 577 J/(kg·K) Show Material materials with Specific heat capacity of 577 J/(kg·K) | ||

500.0 °C | 605 J/(kg·K) Show Material materials with Specific heat capacity of 605 J/(kg·K) | ||

600.0 °C | 648 J/(kg·K) Show Material materials with Specific heat capacity of 648 J/(kg·K) | ||

700.0 °C | 656 J/(kg·K) Show Material materials with Specific heat capacity of 656 J/(kg·K) | ||

800.0 °C | 657 J/(kg·K) Show Material materials with Specific heat capacity of 657 J/(kg·K) | ||

900.0 °C | 657 J/(kg·K) Show Material materials with Specific heat capacity of 657 J/(kg·K) | ||

1000.0 °C | 658 J/(kg·K) Show Material materials with Specific heat capacity of 658 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 14.2 - 17 W/(m·K) Show Material materials with Thermal conductivity of 14.2 - 17 W/(m·K) | |

100.0 °C | 15.5 W/(m·K) Show Material materials with Thermal conductivity of 15.5 W/(m·K) | ||

200.0 °C | 17 W/(m·K) Show Material materials with Thermal conductivity of 17 W/(m·K) | ||

300.0 °C | 18.3 W/(m·K) Show Material materials with Thermal conductivity of 18.3 W/(m·K) | ||

400.0 °C | 19.7 W/(m·K) Show Material materials with Thermal conductivity of 19.7 W/(m·K) | ||

500.0 °C | 20.9 - 23 W/(m·K) Show Material materials with Thermal conductivity of 20.9 - 23 W/(m·K) | ||

600.0 °C | 21.9 W/(m·K) Show Material materials with Thermal conductivity of 21.9 W/(m·K) | ||

700.0 °C | 23.2 W/(m·K) Show Material materials with Thermal conductivity of 23.2 W/(m·K) | ||

800.0 °C | 24.6 W/(m·K) Show Material materials with Thermal conductivity of 24.6 W/(m·K) | ||

900.0 °C | 26.1 W/(m·K) Show Material materials with Thermal conductivity of 26.1 W/(m·K) | ||

1000.0 °C | 27.5 W/(m·K) Show Material materials with Thermal conductivity of 27.5 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 4.2 mm²/s Show Material materials with Thermal diffusivity of 4.2 mm²/s | |

100.0 °C | 3.9 mm²/s Show Material materials with Thermal diffusivity of 3.9 mm²/s | ||

200.0 °C | 3.9 mm²/s Show Material materials with Thermal diffusivity of 3.9 mm²/s | ||

300.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

400.0 °C | 4.1 mm²/s Show Material materials with Thermal diffusivity of 4.1 mm²/s | ||

500.0 °C | 3.2 mm²/s Show Material materials with Thermal diffusivity of 3.2 mm²/s | ||

600.0 °C | 3.9 mm²/s Show Material materials with Thermal diffusivity of 3.9 mm²/s | ||

700.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

800.0 °C | 5.1 mm²/s Show Material materials with Thermal diffusivity of 5.1 mm²/s | ||

900.0 °C | 5.5 mm²/s Show Material materials with Thermal diffusivity of 5.5 mm²/s | ||

1000.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 1.02E-6 - 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.02E-6 - 1.1E-6 Ω·m |

100.0 °C | 1.05E-6 Ω·m Show Material materials with Electrical resistivity of 1.05E-6 Ω·m | |

200.0 °C | 1.09E-6 Ω·m Show Material materials with Electrical resistivity of 1.09E-6 Ω·m | |

300.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

400.0 °C | 1.16E-6 Ω·m Show Material materials with Electrical resistivity of 1.16E-6 Ω·m | |

500.0 °C | 1.2E-6 Ω·m Show Material materials with Electrical resistivity of 1.2E-6 Ω·m | |

600.0 °C | 1.24E-6 Ω·m Show Material materials with Electrical resistivity of 1.24E-6 Ω·m | |

700.0 °C | 1.27E-6 Ω·m Show Material materials with Electrical resistivity of 1.27E-6 Ω·m | |

800.0 °C | 1.28E-6 Ω·m Show Material materials with Electrical resistivity of 1.28E-6 Ω·m | |

900.0 °C | 1.3E-6 Ω·m Show Material materials with Electrical resistivity of 1.3E-6 Ω·m | |

1000.0 °C | 1.31E-6 Ω·m Show Material materials with Electrical resistivity of 1.31E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Aluminium | 1.2 - 1.7 % Show Material materials with Aluminium of 1.2 - 1.7 % |

Carbon | 0.12 % Show Material materials with Carbon of 0.12 % |

Chromium | 23 - 26 % Show Material materials with Chromium of 23 - 26 % |

Manganese | 1 % Show Material materials with Manganese of 1 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.7 - 1.4 % Show Material materials with Silicon of 0.7 - 1.4 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |